Slideshare uses cookies to improve functionality and performance, and to provide you with relevant advertising. If you continue browsing the site, you agree to the use of cookies on this website. See our User Agreement and Privacy Policy.

Slideshare uses cookies to improve functionality and performance, and to provide you with relevant advertising. If you continue browsing the site, you agree to the use of cookies on this website. See our Privacy Policy and User Agreement for details.

Like this presentation? Why not share!

- Hysteresis loop by pancholi aditi 1129 views
- Hysteresis by Sathees Physics 437 views
- B-H curve (hysteresis loop) by Dhruv Dmp 482 views
- Hysteresis and Eddy-current losses by AbdulAziz Ahmed S... 1724 views
- Magnetic Hysteresis by mohammed enab 861 views
- Magnetization curve by Biswajit Pratihari 4247 views

6,466 views

Published on

BH curve hysteresis in ferro ferrimagnets

No Downloads

Total views

6,466

On SlideShare

0

From Embeds

0

Number of Embeds

6

Shares

0

Downloads

0

Comments

0

Likes

11

No embeds

No notes for slide

- 1. B – H Curve : Hysteresis in ferro-/ferrimagnets 1. Diamagnetism – no permanent dipole moment 2. Paramagnetism – permanent non-interacting magnetic dipoles exist 3. Magnetically ordered materials – interaction between moments causes magnetic order leading to ferro-, antiferro- and ferrimagnetism (and non-zero spontaneous magnetization in ferro- and ferrimagnets).
- 2. Types of magnetism 1. Diamagnetism Absence of Permanent magnetic moments Fully filled orbitals On application of magnetic field (H), magnetic moment is induced in such a way to oppose the effect of H Occurs through distortion of orbitals It is proportional to the total no. of electrons . χ dia ~ 10 -6 and is independent of Temperature(T)
- 3. 2. Paramagnetism : Unpaired electrons existing in any orbital Permanent magnetic moments exist on atoms or ions Applied H orients the moments already present, against thermal agitation to randomize them Magnetization M = m/V ; i.e. M is magnetic moment per unit volume Magnetic Susceptibility: ~ 10 -3 = M/H
- 4. Ferromagnetism : M is large M = Ng B J B J (y) ; y = g B H m /k B T Molecular field H m = H + M, is the Weiss molecular field constant B J (y) is the Brillouin function At high T, = C/(T- ) …Curie –Weiss Law At low T, large H : M saturates Induction B = 0 ( H+M) ; Permeability = B/H Antiferromagnetism : M = 0, = C/(T+ ) y
- 5. Magnetic order from T dependence of Susceptibility
- 6. Domain Theory- Competing Energies 1. Magnetostatic energy H d = -N d M ; E d = ( 0 /2)N d M 2 N d is demagnetizing factor 2. Magnetocrystalline energy 3. Exchange Energy J = S i .S J Minimization of total energy leads to formation of domains separated by domain walls. When H is applied, M develops due to movement of Domain walls Irreversible wall motion causes hysteresis and losses
- 7. Anisotropy energy : is due to preference of certain crystallographic directions for the alignment of atomic moments M vs. H for Fe ( Cubic) and Co (Hexagonal) Anisotropy constants Cubic : K Uniaxial : K 1 , K 2 E a = K 1 Sin 2 + K 2 Sin 4 : / M, EA
- 8. Domains and Domain walls 180 0 wall
- 9. B – H hysteresis Curve using an AC Inductance method <ul><li>For a secondary coil of N S turns : = N s A B, A- area of coil </li></ul><ul><li>Emf = - / t = - N S ( B A ) / t = - N S A B / t </li></ul><ul><li>Emf α B / t ; </li></ul><ul><li>H = n p I, n p = N p /l p , No. of turn in primary/unit length </li></ul>This works on the principle of “ Faraday's Law of Induction.” as in Transformers Induced Emf = - / t – from one of the Maxwell’s equations With B , the Magnetic Induction = µ 0 (H+M) , = BA,
- 10. Integrator C R2 R1 P s S s P S Variac Step down Transformer Circuit : V x ( H ) V Y ( B) Sample V x to X – plates of CRO V y to Y- plates of CRO One Primary and one secondary
- 11. Loop Tracer for Toroidal Sample Mutual Inductance set up One primary &Two secondaries – directly gives M – H loops Single primary and single secondary Emf 1 = - N S A µ 0 (H+M) / t Emf 2 = - N S A µ 0 (H) / t
- 12. Hysteresis loops Domain theory : Irreversible motion of domain walls causes hysteresis , large coercivity Presence of defects in domains, domain boundaries causes pinning of the walls & large hysteresis Barkhausen effect - Wall diplacement occurs by jerks
- 13. Barkhausen Effect Cilcks can be heard on a loud speaker Domain walls need to cross potential wells in the magnetization process Flexible Domain Wall - Contributes to Reversible M
- 14. Steps during Magnetization Process H = 0, Random directions of domains Low fields,Reversible Easy dirns. Close to H expand Medium fields, Domains in other equivalent Easy dirns. High fields Domain rotation to H dirn .
- 15. H = 0 Low H Medium H High H
- 16. Formulae : 1. Magnetic field H = n p I in (A/m) ; I = V R /R Here n p = N p /l p - i.e.no. of turns in primary per unit length. N p is the no. of turns in the Primary a) Solenoid : l p = length of primary b) Toroid : l p = 2 r , where r = (r 1 +r 2 ) / 2 r 2 r 1 1 kA/m = 4 Oe,1 Tesla / 0 = 1 A/m 1 T = 10 4 Oe ; 0 = 4 * 10 -7 H / m Toroid
- 17. <ul><li>Magnetic Induction :B = H = 0 ( H + M ) </li></ul><ul><li>Here M is the Magnetization = Magnetic moment / volume </li></ul><ul><li> is the permeability of the sample </li></ul><ul><li> </li></ul><ul><li>Applied current I, as well as M, H and B are time dependent </li></ul><ul><li>in this method. </li></ul>H M T 3 < T 2 < T 1 H B
- 18. where = 2 f where f is the frequency of ac signal used. Here f = 50 Hz ( the line frequency) Secondary Output Let B = B 0 Sin t
- 19. C R 2 R 1 1. To determine the calibration constant of Integrator 2. Measure the value of R in the primary circuit to determine current I, I = V R /R
- 20. Calculate remanance ( B r ), coercivity ( H c ), saturation magnetization ( M s ), field required for saturation ( H s ), Saturation Induction ( B s ) = 4 M s AC Hysteresis loss (W) from the measured B-H curves. The ((1/4 )*area under the B-H curve) gives the information about hysteresis loss in CGS units ( erg / cc / cycle )
- 21. Corrections 1. Demagnetisation The rod shaped ( l / d > 10) and Toroidal shaped samples are chosen to minimize the demagnetizing factors (N) so that H int = H / (1-N) H is a valid approximation. 2. Filling Factor : Here, the sample is assumed to fill the volume of the secondary coil completely. If not, we introduce a Filling Factor ( ) correction which defines the extent of sample filling in the secondary coil.

No public clipboards found for this slide

×
### Save the most important slides with Clipping

Clipping is a handy way to collect and organize the most important slides from a presentation. You can keep your great finds in clipboards organized around topics.

Be the first to comment